MODELING OF THE AGING VISCOELASTIC PROPERTIES OF CEMENT PASTE USING COMPUTATIONAL METHODS

A Thesis by XIAODAN LI

Submitted to the Office of Graduate Studies of Texas A&M University

in partial fulfillment of the requirements for the degree of MASTER OF SCIENCE

May 2012

Modeling of the Aging Viscoelastic Properties of Cement Paste Using Computational Methods

MODELING OF THE AGING VISCOELASTIC PROPERTIES OF CEMENT PASTE USING COMPUTATIONAL METHODS

A Thesis by XIAODAN LI

Submitted to the Office of Graduate Studies of Texas A&M University

in partial fulfillment of the requirements for the degree of MASTER OF SCIENCE

Approved by:

Chair of Committee, *Zachary C. Grasley *
Committee Members, Robert L. Lytton

Anastasia Muliana Head of Department, John M. Niedzwecki

May 2012

ABSTRACT

Modeling of the Aging Viscoelastic Properties of Cement Paste Using Computational Methods. (May 2012)

Xiaodan Li, Be.N., Hong Kong University of Science and Technology Chair of Advisory Committee: Dr. Zachary Grasley

Modeling of the time-dependent behavior of cement paste has always been a difficulty. In the past, viscoelastic behavior of cementitious materials has been primarily attributed to the viscoelastic properties of C-S-H components. Recent experimental results show that C-S-H may not exhibit as much creep and relaxation as previously thought. This requires new consideration of different mechanisms leading to the viscoelastic behavior of cement paste. Thus the objective of this thesis is to build a computational model using finite element method to predict the viscoelastic behavior of cement paste, and using this model, virtual tests can be carried out to improve

understanding of the mechanisms of viscoelastic behavior.

The primary finding from this thesis is that the apparent viscoelastic behavior due to dissolution of load bearing phases is substantial. The dissolution process occurring during the hydration reaction can change the stress distribution inside cementitious materials, resulting in an apparent viscoelastic behavior of the whole cementitious materials. This finding requires new consideration of mechanisms of

ACKNOWLEDGEMENTS

I would like to express my gratitude to all those who helped me in completing this report. First I must give my special thanks to my supervisor Dr. Grasley for his continual encouragement, technical and personal guidance. I also want to thank my committee members, Dr. Lytton and Dr. Muliana, for their guidance and support throughout this research. My friend, Christopher A. Jones and Ardavan Yazdanbakhsh gave me a lot of help when I came across difficulties. Additionally, I would like to thank Dr. E.J. Garboczi and Dr. Jeffrey Bullard for their technical support on the research. Without their support, there is no way I can finish this work. I really appreciate all your guidance, help and patience.

Thanks to the Zachry Department of Civil Engineering of Texas A&M

University for giving me the opportunity to start working on this project in the first place, providing me necessary environment to carry out this project and allowing me to use all resources.

Finally, thanks to my mother and my father for their encouragement and support. I love you.

C-S-H calcium silicate hydrate

*E * elastic Young‟s modulus

*E(t) * apparent viscoelastic Young‟s modulus

*K * elastic Bulk modulus

*K(t) * apparent viscoelastic Bulk modulus

*G * elastic Shear modulus

*G(t) * apparent viscoelastic Shear modulus

𝜐 elastic Poisson‟s ratio

𝜐 𝑡 apparent viscoelastic Poisson‟s ratio

*w/c * water to cement mass ratio

*t * time

𝑆𝑖𝑗𝑘𝑙 viscoelastic compliance tensor

𝜎 stress

𝜀 strain

𝐶_{𝑖𝑗𝑘𝑙} elastic moduli tensor

*A * Hessian matrix

*u * displacement

*gb * energy gradient

𝜌 mass density

Page

ABSTRACT ... iii

ACKNOWLEDGEMENTS ... v

NOMENCLATURE ... vi

TABLE OF CONTENTS ... viii

LIST OF FIGURES ... xi

LIST OF TABLES ... xiv

CHAPTER I INTRODUCTION ... 1

1.1 Motivation ... 1

1.2 Scope and Problem Statement ... 3

1.3 Tasks ... 4

1.4 Disposition ... 4

CHAPTER II LITERATURE REVIEW ... 6

2.1 Viscoelastic Properties of Aging Cement Paste ... 6

2.1.1 General ... 6

2.1.2 Viscoelastic Properties of C-S-H ... 7

2.1.3 Hydration Process ... 9

2.2 Current Viscoelastic Constitutive Models ... 11

2.2.1 General Constitutive Theory ... 11

2.2.2 Solidification Theory ... 12

2.2.3 Mathematical and Physical Representation of Modulus and Compliance ... 14

2.3 Linear Elastic Model Using Finite Element Method ... 16

Page

2.3.2 Linear Elastic Composite Model ... 17

2.4 Hydration Model ... 23

2.5 Viscolasticity of C-S-H ... 23

CHAPTER III COMPUTER MODELING THEORY ... 26

3.1 Elastic ... 26

3.2 Viscoelastic ... 27

3.1.2 Theory ... 27

3.2.2 Flow Chart ... 31

3.3 Dissolution and Formation ... 33

3.3.1 Theory ... 33

3.3.2 Flow Chart ... 35

CHAPTER IV RESULTS AND DISCUSSION ... 37

4.1 Validation of Model ... 37

4.1.1 Elastic ... 37

4.1.2 Viscoelastic ... 39

4.1.3 Dissolution-Formation ... 40

4.2 Viscoelasticity of C-S-H and Hydration ... 43

4.2.1 Viscoelasticity of C-S-H ... 45

4.2.2 Viscoelasticity of C-S-H and Dissolution ... 48

4.2.3 Mechanisms of Viscoelasticity of Cement Paste ... 50

4.3 Predicted Effect of Different Loading Ages ... 51

4.3.1 Apparent Viscoelastic Young‟s Modulus... 51

4.3.2 Rate of Relaxation ... 53

4.4 Predicted Effect of Different w/c ... 54

4.4.1 Apparent Viscoelastic Young‟s Modulus... 54

4.4.2 Rate of Relaxation ... 57

4.5 Predicted Stress Distribution ... 66

4.5.1 Volumetric Stress and Deviatoric Stress ... 66

4.5.2 Comparison between Dissolution-Formation Viscoelastic Model and Solidification Theory ... 70

CHAPTER V CONCLUSION AND FUTURE WORK ... 74

5.1 Conclusion ... 74

5.2 Future Work ... 76

REFERENCES ... 78

APPENDIX A ... 82

LIST OF FIGURES

Page Figure 1 Mechanisms of Viscoelastic Behavior of Cementitious Materials. ... 7 Figure 2 Typical Creep Curve for Plain Concrete ... 8 Figure 3 Schematic Outline of Microstructure Development in Portland Cement

Pastes ... 10 Figure 4 Conceptual Diagram of Solidifying Material Subjected to Applied

Stress ... 13 Figure 5 The Kelvin Chain and the Maxwell Chain ... 15 Figure 6 Complete Flow Chart for Finite Element Linear Elastic Composite

Model. ... 21 Figure 7 Simplified Flow Chart for Finite Element Linear Elastic Composite

Model. ... 22 Figure 8 Uniaxial Viscoelastic Compliance of C-S-H Measured Using

Experimental Methods ... 24 Figure 9 Virtual Work Demonstration. ... 28 Figure 10 Flow Chart for Linear Viscoelastic Model. ... 32 Figure 11 Conceptual Diagram of Computational Model Simulating Apparent

Viscoelastic Behavior of Hydrating Cement Paste ... 33 Figure 12 Flow Chart for Dissolution-Formation Viscoelastic Model. ... 36 Figure 13 Comparison of Elastic Results from the Dissolution-Formation

Viscoelastic Program, the NISTIR ELAS3D Program and the Abaqus

Program ... 38 Figure 14 Comparison of Viscoelastic Results from the Dissolution-Formation

Viscoelastic Program and the Abaqus Program ... 40 Figure 15 Virtual Applied Strain History. ... 41

Figure 16 Response of Aging Viscoelastic Composite Material when a Strain History Shown in Figure 15 is Applied. ... 42 Figure 17 Viscoelastic Young‟s Modulus for Cement Paste at Different Ages

when Dissolution and Formation Effect is not Considered ... 46 Figure 18 Response of Cement Paste with an Assumed Viscoelastic Young‟s

Modulus of C-S-H Comparing to the Response of Cement Paste when C-S-H is Considered Elastic. ... 49 Figure 19 Apparent Viscoelastic Young‟s Modulus of 0.40 w/c Paste when

Loaded at Different Ages ... 52 Figure 20 Effect of Initial Loading Age on Normalized Apparent Viscoelastic

Relaxation ... 53 Figure 21 Apparent Viscoelastic Young‟ Modulus for Different w/c at Loading

Age of 1 Day ... 55 Figure 22 Apparent Viscoelastic Young‟ Modulus for Different w/c at Loading

Age of 7 Days ... 56 Figure 23 Effect of Different w/c on Normalized Apparent Viscoelastic

Relaxation at Loading Age of 1 Day ... 57 Figure 24 Effect of Different w/c on Normalized Apparent Viscoelastic

Relaxation at Loading Age of 7 Days. ... 58 Figure 25 Effect of Different w/c on Viscoelastic Relaxation at Loading Age

of 1 Day ... 59 Figure 26 Apparent Viscoelastic (a) Bulk Modulus, (b) Shear Modulus and (c)

Poisson‟s Ratio Results for Different w/c at Loading Age of 1 Day ... 61 Figure 27 Apparent Viscoelastic (a) Bulk Modulus, (b) Shear Modulus and (c)

Poisson‟s Ratio Results for Different w/c at Loading Age of 7 Days ... 63 Figure 28 Normalized Volumetric Stress and Deviatoric Stress Carried by

Hydrated Phases and Unhydrated Phases inside Cement Paste

Page Figure 29 Comparison between the Dissolution-Formation Viscoelastic Model

and the Solidification Theory on Normalized Volumetric Stress Carried by Solidified Phases. ... 71 Figure 30 Comparison between the Dissolution-Formation Viscoelastic Model

and the Solidification Theory on Normalized Deviatoric Stress Carried by Solidified Phases. ... 72

Page Table 1 Elastic Moduli of Individual Cement and Cement Paste Phases ... 17

CHAPTER I INTRODUCTION

**1.1 Motivation **

The mechanical properties of cement-based materials, which play a key role in civil infrastructure, have been studied for a long time. Studies have been carried out in developing numerical computational methods to predict their linear elastic properties [1]. However, in reality, cementitious materials are viscoelastic, and to accurately predict stress and strain in cementitious materials, proper understanding of the viscoelastic behavior is necessary. Portland cement concrete by far is the most used construction material worldwide because of its many advantages [2]; thus, understanding the mechanical constitutive behavior of cementitious materials is important for predicting stress and strain in infrastructure.

There are currently several theories that attempt to explain the viscoelastic behavior of cement-based materials, but none of them are capable of describing the viscoelastic behavior adequately. One reason for this is that cement-based materials are composite materials with random matrix arrangement, which are difficult to model; another reason is that the internal chemical components of cement-based materials are changing during the hydration process [3], including dissolution of existent components and forming of new components. The forming of new components in cementitious ____________

aging occurring in other viscoelastic materials, in this thesis, the aging process is specified only as the hydration process inside cementitious materials, in which the materials gradually stiffen and their relaxation rates slow down as it “cures” [4].

Viscoelastic behavior of cementitious materials has been primarily attributed to the viscoelastic properties of C-S-H components inside cementitious materials [5]. However, in recent experiments, the results indicate that C-S-H may not exhibit as much creep and relaxation as previously thought [6]. This requires new consideration of different mechanisms leading to the viscoelastic behavior of cement paste. By modeling cement paste‟s aging viscoelastic behavior, virtual computational experiments can be carried out, and through analyzing the modeling results, the mechanisms causing the viscoelastic behavior of cement paste may be elucidated.

To effectively model cement paste‟s aging viscoelastic properties, an analytical constitutive model of cement paste based on microstructure can be built, and then the inherent, aging viscoelastic behavior of the micrometric cement paste phases can be integrated to predict the macroscale viscoelastic responses of cement paste.

Through the modeling of aging viscoelastic properties of cement paste, a fundamental understanding of the time dependent behavior of concrete can be reached. In the future, the computational model developed in this research may be used in predicting the behavior of concrete by engineers and to help improve the design of damage-resistant structures. It may also assist in overcoming the current limitations of concrete and developing new advanced materials.

**1.2 Scope and Problem Statement **

Current limitations with predicting the aging viscoelastic properties of cement paste are that:

There is no current ability to predict viscoelastic constitutive properties based on cement characteristics;

There are models linking observed viscoelastic behavior with evolving microstructure linked to hydration process.

The goal of this master‟s thesis is to:

Develop a qualified aging viscoelastic composite model for predicting aging viscoelastic properties of cement paste;

Better understand the mechanisms of viscoelastic behavior through running virtual experiments using the newly developed computational model.

To develop the computational aging viscoelastic composite model, the programming language C++was used with the computational compiling software Microsoft Visual Studio. Since this aging viscoelastic model was a modification of the linear elastic composite materials model developed by Garboczi et al. in the

programming language Fortran [1], at the beginning of this project, the programming language Fortran and its compiling software Fortran Powerstation was mainly used.

This thesis research project can be divided into several phases: Review Literature;

Transfer the existent linear elastic model from Fortran to C++; Convert the linear elastic model to a viscoelastic model;

Further develop the model to simulate the dissolution-formation process of cement-based materials;

Check the accuracy of the finalized model; Run virtual experiments and analysis;

Draw conclusions from virtual experiments regarding mechanisms of viscoelastic behavior of cementitious materials.

**1.4 Disposition **

This report consists of five chapters. Chapter 2 reviews the previously

hypothesized mechanisms for the viscoelastic behavior of cement paste, along with an existent aging viscoelastic model which has some limitations in predicting the behavior of cement paste. Overview of the three dimensional linear elastic model ELAS3D is also included in this chapter. Chapter 3 develops the dissolution-formation viscoelastic model and describes the model in flow charts. Chapter 4 presents the results from the model and includes some discussions and comparisons related to the results. Chapter 5

of these chapters. The appendix contains the program code for the dissolution-formation viscoelastic model. Equation Chapter (Next) Section 1

LITERATURE REVIEW

In this chapter, hypothesized mechanisms of viscoelastic behavior of cement paste, together with current models are reviewed. In addition, the finite element method and a computational hydration model, which are the basis for developing a qualified aging viscoelastic model, are also reviewed. Equation Chapter (Next) Section 1

**2.1 Viscoelastic Properties of Aging Cement Paste **

**2.1.1 General **

There are two different aspects leading to the comprehensive viscoelastic behavior of cement paste, as shown in Figure 1:

First, cement paste‟s viscoelastic properties are often subdivided into two types: basic components and drying components, which are also referred as „basic creep‟ and „drying creep‟. Basic creep is creep in the absence of drying, while drying creep is the additional creep that occurs during drying.

Another critical aspect of viscoelastic behavior of cement paste is the hydration process. During the hydration process, there are changes in internal structure leading to changes in stress and strain distribution. The hydration process can also be divided into two different parts: dissolution and formation. Because of dissolution, the inherent stress will redistribute after dissolution of loaded unhydrated phases and the responses of new

formed components critically depend on load histories relative to the time they are “formed”.

*Figure 1 Mechanisms of viscoelastic behavior of cementitious materials. *

**2.1.2 Viscoelastic Properties of C-S-H **

Creep is the tendency of a solid material to deform over some time under the influence of constant stresses. Although all real materials undergo some time-dependent deformation under load, cement paste exhibits larger time-dependent deformation than some other materials, such as ceramics and metals. This is because the fundamental origins for creep of cement paste are different from other materials. In the past, the origins of creep are primarily attributed to the response of C-S-H to stress. Figure 2 shows the typical creep responses of cement-based materials.

Viscoelastic Behavior of Cementitious Materials

Viscoelasticity of C-S-H Hydration Process

*Figure 2 Typical creep curve for plain concrete [5]. *

There are several proposed mechanisms of viscoelastic behavior of cement paste found in the literature:

Seepage of physically bound water (within the layers of C-S-H) into capillary water as a result of external load, which is also known as the seepage theory (by Powers) [7, 8];

Crystallization of C-S-H forming new interlayer space (introduced by Feldman and Sereda) [7, 9];

Sliding of C-S-H globules or layers under localized nanoscale shear stresses ( the viscous shear theory) [7, 10];

**2.1.3 Hydration Process **

Another critical aspect of viscoelastic behavior of cement paste is the hydration process. Hydration occurs independently of the application of external forces. It is a result of the chemical and physical processes that take place between cement and water. The hydration process causes an inherent component change, and thus the responses of cementitious materials to loads critically depend on load histories relative to the time the new components are “formed” [4].

The main hydration reaction is the reaction between tricalcium silicate and water and between dicalcium silicate and water, and the principal hydration product is C-S-H together with calcium hydroxide. As the hydration process continues, more and more C-S-H is produced and less and less of the silicate phases are left.

Figure 3 illustrates the inherent microstructure change during the hydration process.

*Figure 3 Schematic outline of microstructure development in Portland cement pastes: (a) *
*initial mix; (b) 7 days; (c) 28 days; (d) 90 days. (Calcium sulfoaluminates are included *
*as part of C-S-H for simplification) [5]. *

As previously shown in Figure 1, the hydration process can be divided into two parts: (a) dissolution of loaded unhydrated phases and (b) forming of new components.

Dissolution of load bearing phases has been proposed as one potential mechanism for the time-dependent deformation of cementitious materials [11]. Mechanisms regarding the aging process have also been considered. Bazant et al. suggested that the microprestress-solidification process appears to be another creep mechanism [7, 12]. The microprestress is generated by disjoining pressure of the hindered adsorbed water in the micropores and by large localized volume changes

caused by hydration. Irreversible creep can be closely related to the aging process due to silicate polymerization induced by drying [7, 13].

**2.2 Current Viscoelastic Constitutive Models **

Cement paste is known to exhibit time-dependent deformation under different stress histories. A significant amount of research has been carried out to develop valid mathematical models to fit the viscoelastic behavior of viscoelastic materials, and several simple constitutive models have been successfully utilized, such as the Maxwell model, the Kelvin-Voigt model, and the Standard Linear Solid Model [4].

All these models can show accurate simulations for a linear viscoelastic material under different forms of stresses, but the effect of hydration reaction on creep of

concrete is not considered in these models. A popular theory which combines linear viscoelasticity and the formation effect is the solidification theory [14, 15], and it will be introduced in detail later in this chapter.

**2.2.1 General Constitutive Theory **

The most general form of the constitutive equation for a linear viscoelastic
material is
𝜀_{𝑖𝑗} 𝑡 = 𝑆𝑖𝑗𝑘𝑙
𝑡
𝑜
𝑡 − 𝑡′ 𝜕𝜎𝑘𝑙(𝑡′)
𝜕𝑡′ 𝑑𝑡′ + 𝜀𝑓(𝑡)𝛿𝑖𝑗*, * (2.1)

the free strain, 𝜀_{𝑖𝑗} 𝑡 is the overall time-dependent strain, and 𝛿_{𝑖𝑗}* is Kronecker‟s delta. In *
this equation, 𝑆_{𝑖𝑗𝑘𝑙}(𝑡) is a function of single variable 𝑡 − 𝑡′_{ . }

For aging linear viscoelastic materials, the most general form is

𝜀_{𝑖𝑗} 𝑡 = 𝑆_{𝑖𝑗𝑘𝑙}
𝑡
𝑜

𝑡，𝑡′ 𝜕𝜎𝑘𝑙(𝑡′)

𝜕𝑡′ 𝑑𝑡′ + 𝜀𝑓 𝑡 𝛿𝑖𝑗*, * (2.2)
where 𝑆_{𝑖𝑗𝑘𝑙}*(𝑡) is a function of both t and 𝑡*′_{. Some well-known constitutive models }
coupling the viscoelasticity and aging effect are essentially different forms of eq. (2.2),
such as the time-shift theory and the solidification theory [16].

**2.2.2 Solidification Theory **

The solidification theory is a theory accounting for the formation effect on creep of concrete. This theory implies that hydration products are non-aging viscoelastic materials and aging presents in the bulk scale due to the increase in load bearing materials as a result of solidification and deposition of hydration products [17]. As hydration progresses, each newly-formed layer of the hydration products solidifies in a stress-free state and these layers are only subject to loads after they form. This theory is shown conceptually in Figure 4.

*Figure 4 Conceptual diagram of solidifying material subjected to applied stress, 𝜎. The *
*volume of solidified gel is dependent on the aging function 𝜐 𝑡 (which is representative *
*of the volume of load-bearing products that have formed) and 𝜎*𝑔*(𝑣, 𝑡) is the stress *
*distribution carried by solidified phases depending on the aging function and time [15, *
*16]. *

According to the solidification theory, the constitutive equation for a uniaxial
load is
𝜕𝜀11(𝑡)
𝜕𝑡 =
𝐽0
𝜈(𝑡)
𝜕𝜎11(𝑡)
𝜕𝑡 +
1
𝜈(𝑡)
𝜕𝐽_{𝑔}(𝑡 − 𝑡′_{)}
𝜕𝑡′
𝜕𝜎11(𝑡′)
𝜕𝑡′ 𝑑𝑡′
𝑡
0
*, * (2.3)

Where 𝐽_{0}* 𝑖s the instantaneous elastic uniaxial compliance*, 𝜎_{11}(𝑡) is the applied uniaxial
*stress at time t, 𝜈(𝑡) is the aging function and 𝐽*𝑔(𝑡 − 𝑡′) is the non-aging viscoelastic
uniaxial compliance [14].

Another form of the constitutive equation for a solidifying, linear viscoelastic material is expressed as:

𝜎11 𝑡 = 𝜈 𝑡′ _{𝜕𝑡}_{′} 𝐸𝑔 𝑡 − 𝑡′ 𝑑𝑡′
0−

*, * (2.4)

where 𝜈(𝑡) is the aging function, 𝐸𝑔(𝑡 − 𝑡′*) is the non-aging viscoelastic uniaxial *
moduli of the solidifying phases [18].

The solidification theory has a significant limitation when applied to concrete.
For cementitious materials, formation of new load bearing phases (such as C-S-H)
requires dissolution of existing loading bearing phases (such as tricalcium silicate). The
solidification theory predicts the formation process well but it does not consider the
dissolution of existing load bearing phases, as a result, the stress carried by new load
bearing phases is gradually decreasing according to solidification theory. However,
when accounting for dissolution, load is transferred gradually from unhydrated phases to
*newly formed phases and the stresses carried by these new phases are increasing. A *
detailed comparison between the solidification theory and the dissolution-formation
viscoelastic model developed in this thesis will be shown in Chapter 4.

**2.2.3 Mathematical and Physical Representation of Modulus and Compliance **

As mentioned at the beginning of this chapter, there are many mathematical models that can simulate the moduli of linear viscoelastic materials. Two of the most popular forms are the Kevin chain and the Maxwell Chain, which are shown in Figure 5.

The formula for expressing the Kevin chain is

𝐽 𝑡 = 1
𝑅𝑖 1 − 𝑒
−𝑡
𝜏𝑖_{ ,}
𝐼
𝑖=1
(2.5)

where 𝐽 𝑡 is the viscoelastic compliance of the whole system, 𝜏𝑖 = 𝜂𝑖/𝑅𝑖* are called the *
retardation times, 𝑅𝑖* is the elastic Young‟s modulus of spring i in the model and 𝜂*𝑖 is the
*viscosity coefficient of damper i [4]. *

The formula for expressing the Maxwell chain is

𝐸 𝑡 = 𝑅𝑖(𝑒−
𝑡
𝜏𝑖_{)}
𝐼
𝑖=1
*, * (2.6)

where 𝐸 𝑡 is the viscoelastic Young‟s modulus of the whole system, 𝜏_{𝑖} = 𝜂_{𝑖}/𝑅_{𝑖}* are the *
relaxation times, 𝑅𝑖* is the elastic Young‟s modulus of spring i in the model and 𝜂*𝑖 is the
*viscosity coefficient of damper i [4]. *

*Figure 5 The Kelvin Chain (a.) and the Maxwell Chain (b.) [16]. 𝑅*_{𝑖}* are springs’ *
*Young’s modulus and 𝜂*_{𝑖}* are dampers’ viscosity coefficients. *

Since the Kelvin Chain is ideal for modeling creep and the Maxwell Chain is ideal for modeling stress relaxation, for the dissolution-formation viscoelastic model in

used.

**2.3 Linear Elastic Model Using Finite Element Method **

**2.3.1 Finite Element Method **

The finite element method is a general technique for constructing approximate solutions to boundary-value problems [19].

The finite element method is the solution technique used for both elastic models and viscoelastic models presented in this thesis. It involves dividing the domain of a solution into a finite number of simple subdomains, and constructing an approximation of solution over the collection of finite elements.

Thus, for a macro-scaled cement paste microstructure, the 3D composite is divided into a finite number of micro-scaled voxels, and each voxel has its own mechanical properties due to the complexity of cement-based materials. Numerical analysis is carried out on these finite number of voxels. When boundary conditions are applied, for example, a fixed load applied on the boundary of the microstructure, voxels will deform according to the load. Using the finite element method, the displacement of each voxel can be calculated, and thus the total composite mechanical response of the whole microstructure.

**2.3.2 Linear Elastic Composite Model **

There is currently a linear elastic composite model developed by Garboczi et al. [1, 20, 21] for predicting the linear elastic behavior of cement paste using the finite element method. This three dimensional elastic model is also referred to as the ELAS3D model.

The hydration model CEMHYD3D is used to generate the microstructure for this
ELAS3D model at the micrometer length scale. The output of the CEMHYD3D model
is a 3-D digital microstructure where each voxel is labeled with a single phase at the
*dimension of 1 𝜇𝑚*3_{. ELAS3D treats each cubic voxel as a tri-linear finite element and }
the elastic equations are solved using a relaxation algorithm [22].

In this finite element model, elastic moduli for each voxel used are shown in Table 1.

*For an isotropic elastic material, with any two of the set: the Young‟s modulus, E, *
the Poisson‟s ratio, ν, the Bulk modulus, K, and the Shear modulus, G, the remaining
two elastic moduli can be calculated through

𝐾 = 𝐸

3 1 − 2𝜈 𝐺 = 𝐸

2 1 + 𝜈 *. * (2.7)

These equations can be used to solve elastic moduli with different known combinations of these parameters [23, 24].

The ELAS3D model is a strain controlled model with periodic boundary
conditions. Strain controlled means that the bulk strain applied on the whole system is
kept constant and periodic boundary conditions mean that if there is a neighbor outside
the digital image, the model is periodically continued on the opposite side of the system.
*2.3.2.1 Theory *

The theory on which the finite element program ELAS3D is based is simple. For a given microstructure under applied boundary conditions, such as a controlled strain, the final displacement distribution is calculated such that the total energy stored in the elastic microstructure is minimized. Another way of expressing the essential idea of this finite element program is that the gradient of energy with respect to elastic displacement is zero:

*𝐺𝑟𝑎𝑑(𝐸𝑛) = 0, * (2.8)

In this finite element program, the sum of the squares of the gradient vector of all elements is forced to be less than a prescribed small value, so that the condition

expressed in eq. (2.8) is approximately satisfied.

For an elastic microstructure, the total elastic energy is given by

𝐸𝑛 =1
2 𝜀𝑝𝑞𝐶𝑝𝑞𝑟𝑠𝜀𝑟𝑠𝑑𝑥 𝑑𝑦 𝑑𝑧
1
0
1
0
1
0
*, * (2.9)

*where 𝜀*_{𝑝𝑞} is the strain tensor and 𝐶_{𝑝𝑞𝑟𝑠}* is the elastic moduli tensor, p, q, r, s = 1, 2, or 3, *
and the integral is over the volume of a single unit voxel.

By expressing the strain tensor in terms of displacement components, eq. (2.9) can be rewritten as

𝐸𝑛 = 1

2𝑢𝑟𝑝𝑇 𝐷𝑟𝑝𝑠𝑞𝑢𝑠𝑞*, * (2.10)

where 𝐷_{𝑟𝑝𝑠𝑞} is the stiffness matrix and 𝑢_{𝑟𝑝}* is the p‟th component of displacement at r‟th *
node.

Since periodic boundary conditions are applied, for a voxel at the boundary,
displacement of its nodes: 𝑢_{𝑟𝑝} = 𝑈_{𝑟𝑝} + 𝛿_{𝑟𝑝}, where 𝑈_{𝑟𝑝} is the displacement vector
determined by surrounding voxels and 𝛿_{𝑟𝑝} is the correction vector determined by
boundary conditions.

Inserting these boundary conditions, the expression for energy becomes

𝐸𝑛 =1

2 𝑢𝑟𝑝𝑇 𝐷𝑟𝑝 ,𝑠𝑞𝑢𝑠𝑞 + 2𝛿𝑟𝑝𝐷𝑟𝑝 ,𝑠𝑞𝑢𝑠𝑞 + 𝛿𝑟𝑝𝐷𝑟𝑝 ,𝑠𝑞𝛿𝑠𝑞* , * (2.11)
which can be simplified as

*where A is the Hessian matrix composed of the stiffness matrices, b is a constant vector *
*and C is a constant that is determined by the applied strain and periodic boundary *
*conditions, and u is a vector of all the displacements. *

*The only contributions to b and C come from voxels having nodes at the unit cell *
*boundaries and having a non-zero stiffness matrix. In other words, b and C are *

determined by boundary conditions.

When integrating the energy inside each voxel, since there is no term to be integrated that is higher order than quadratic, Simpson's rule is used for solving the exact solution of the quadratic functions.

The solution method used is the conjugate gradient relaxation algorithm: 𝜕𝐸𝑛

𝜕𝑢 *= 𝑔𝑏 𝑔𝑟𝑎𝑑𝑖𝑒𝑛𝑡 = 𝐴𝑢 + 𝑏. * (2.13)

*By changing the values of u, the final results of u can be found when *

𝑔𝑔 = 𝑔𝑏 ∗ 𝑔𝑏 is close enough to zero or when the program has been run enough times.
*When gg is close enough to zero, it means that the total energy of the system approaches *
a minimum.

*2.3.2.2 Flow Chart *

*Figure 6 Complete flow chart for finite element linear elastic composite model. *

**YES**

**Calculate averaged stress **
**and strain, output modulus **

**END **

**Input material properties **
**for each voxel and apply **
**controlled strain **

**Calculate Hessian matrix **
**(A), calculate boundary **
**condition (b and C) **

**Calculate energy and **
**gg=gb*gb **

**Set initial displacement **
**for each node (u) **

**Is gg small **
**enough? **
**Set material **

**dimension **
**Start **

**Change the values of **
**displacements (u) **

**Have the loop been **
**run enough times? **

**YES **
**NO**

*Figure 7 Simplified flow chart for finite element linear elastic composite model. *
**NO **

**Input basic information of the **
**material and calculate all **
**necessary matrixes **

**Calculate energy **
**Set initial displacement **
**for each node (u) **

**Is ** **energy **
**minimized? **

**Start **

**Calculate ** **and ** **output **
**modulus **

**Change the values of **
**displacements u **

**END **
**YES **

**2.4 Hydration Model **

In this thesis, instead of CHMHYD3D model, a complementary numerical model called THAMES [25, 26] is used to simulate the system of cement hydration and

microstructure development. It relies heavily on equilibrium thermodynamic calculations to predict the assemblage of phases and then using a digital image representation, it distributes these phases into a 3D microstructure model.

To predict time-dependent phase assemblage in hydrating cement pastes,

equilibrium thermodynamic calculations coupled with a kinetic model for the dissolution rates have been used. Combining this approach with a lattic-based 3D microstructure model, microstructure development during the hydration process can be simulated. This is the basis for the THAMES model. Using the finite element method on one 3D microstructure image, as shown in this thesis, effective elastic and viscoelastic moduli can be calculated [25-27].

**2.5 Viscolasticity of C-S-H **

C-S-H has different mechanical properties on the nanometric scale versus on the micro scale by different test results based on AFM (atomic force microscopy) tests and nanoindentation measurements. [28-30]

*Figure 8 Uniaxial viscoelastic compliance of C-S-H measured using a traditional *
*nanoindenter and an AFM; values are normalized by instantaneous uniaxial compliance *
*and vertical bars indicate one standard deviation [31]. *

The measured uniaxial viscoelastic compliances of cement paste measured using both nanoindenter and AFM are shown in Figure 8. Measurements with the

nanoindenter yield a higher creep rate than measurements performed with an AFM. A possible explanation for the higher creep rate exhibited in the nanoindenter test is that multiple creep processes are present in the nanoindenter test, while only inherent viscoelasticity of C-S-H is present in the AFM test because of its smaller test volume. The nanoindenter is more likely probing multiple phases (both hydrated and unhydrated) simultaneously [32, 33]. Thus, Figure 8 suggests that, since more creep is observed with a larger volume of material interacted, C-S-H viscoelasticity cannot be the sole

1 1.1 1.2 1.3 1.4 0 5 10 15 20 25 30 Nanoindenter AFM J(t)/J(0) Time (s)

mechanism behind bulk (e.g. meter scale) viscoelastic response of cementitious materials.Equation Chapter (Next) Section 1

CHAPTER III

COMPUTER MODELING THEORY

This chapter describes the theory and steps to develop a qualified dissolution-formation viscoelastic model using the finite element method. Model inputs and flow chart of the simulation program are shown in detail in this chapter.

The development of the computational dissolution-formation viscoelastic model contains three main parts: (1) build a linear elastic composite model using C++; (2) modify the linear elastic composite model so that it can simulate the behavior of linear viscoelastic composite materials; (3) further develop the finite element model to predict the dissolution-formation viscoelastic behavior of cement paste. Through the whole program, the elastic moduli used for different phases are shown in Table 1.

**3.1 Elastic **

The elastic model developed in this research is the same as the linear elastic composite model ELAS3D. The program was transformed from Fortran to C++, because the programming language C++ is more flexible and is capable of more complex

calculations.

The elastic program shows the same calculation theory and flow chart as the linear elastic program shown in Chapter 2.

**3.2 Viscoelastic **

Modification of the elastic program is needed for the program to predict the viscoelastic behavior of composite materials. It is known that viscoelastic response is a long-term history-dependent response. Different load histories lead to different

responses. To accurately predict cement paste‟s viscoelastic properties, the concept of time steps is used in the model. This model divides a continuous time into a finite

number of discrete time steps and assumes the modulus of C-S-H to stay constant during each time step. In this way, the viscoelastic problem can be solved at different time steps, and simulation of viscoelastic behavior becomes achievable.

**3.1.2 Theory **

As mentioned in section 2.3, the main method for finding the inherent displacement and stress fields in the finite element method is to minimize the total energy stored inside the whole microstructure. Since viscoelastic response is not a static response, to calculate the energy of microstructure, the principle of virtual work or virtual velocities, demonstrated in Figure 9, can be used to derive the equation expressing the energy of viscoelastic materials.

*3.1.2.1 Virtual Work *

In this model, the derived energy equation is assumed to be applied under a quasi-static state with a negligible inertial. Depending on this, the derivation of the energy equation is shown below:

*Figure 9 Virtual work demonstration [34]. *

Consider a solid with mass density 𝜌, the equilibrium equation for balance of linear momentum is

𝜎_{𝑗𝑖 ,𝑗} + 𝑏_{𝑖} = 𝜌𝑢_{𝑖}* , 𝑖, 𝑗 = 1,2,3 * (3.1)
where 𝜎_{𝑗𝑖 ,𝑗} are components of Cauchy Stress [35, 36], 𝜌 is mass density, 𝑏_{𝑖} are body
force components and 𝑢_{𝑖} are displacement components.

According to balance of angular momentum, 𝜎𝑗𝑖 = 𝜎𝑖𝑗.

For all points in the domain of the problem 𝛺, stress boundary conditions are given by

𝑡_{𝑖} = 𝜎_{𝑗𝑖}𝑛_{𝑗} = 𝑡* *_{𝑖} (3.2)

for all points lying on the boundary 𝑆2.

From the virtual work principle, the total work done by external forces are

𝛿𝑢_{𝑖}𝑏_{𝑖}𝑑𝛺
𝛺

+ 𝛿𝑢_{𝑖}𝑡 𝑑𝛺_{𝑖}
𝑆2

where, as mentioned above, 𝛺 is the domain of the problem and 𝑏𝑖 are body force components.

For the work change inside the material, one component is the change of kinetic energy, the other component is the work done by Cauchy stresses, which is either dissipated as heat or stored as internal energy. This change is

𝛿𝑢_{𝑖}𝜌𝑢_{𝑖} 𝑑𝛺
𝛺

+ 𝛿𝜖_{𝑖𝑗}𝜎_{𝑖𝑗}𝑑𝛺
𝛺

*, * (3.4)

where 𝛿𝜖_{𝑖𝑗} =1_{2} 𝛿𝑢_{𝑖,𝑗} + 𝛿𝑢_{𝑗 ,𝑖} for infinitesimal displacement gradients.
These terms in eq. (3.3) should be equal to those in eq. (3.4), thus:

𝛿𝑢𝑖𝑏𝑖𝑑𝛺
𝛺
+ 𝛿𝑢𝑖𝑡 𝑑𝛺𝑖
𝑆2
− 𝛿𝑢𝑖𝜌𝑢𝑖 𝑑𝛺
𝛺
− 𝛿𝜖𝑖𝑗𝜎𝑖𝑗𝑑𝛺
𝛺
*= 0. (3.5) *
As mentioned at the beginning of this section, for long-term relaxation

simulation, the velocity can be approximated as zero, thus eq. (3.5) becomes

𝛿𝑢_{𝑖}𝑏_{𝑖}𝑑𝛺
𝛺
+ 𝛿𝑢_{𝑖}𝑡 𝑑𝛺_{𝑖}
𝑆2
− 𝛿𝜖_{𝑖𝑗}𝜎_{𝑖𝑗}𝑑𝛺
𝛺
*= 0. * (3.6)

The above equation can be rewritten as:

𝛿𝑢𝑏𝑑𝛺 𝛺

+1

2 𝛿𝑢𝜎𝑑𝛺_{𝛺} = 𝛿𝜀𝜎𝑑𝛺_{𝛺} *, * (3.7)

since for small deformation, 𝛿𝑢_{𝑟} *= 𝜀, where r is the dimension of one voxel, which equals *
one, thus 𝛿𝑢 = 𝜀 and eq. (3.7) becomes

𝐸𝑛 ≈ 𝑏𝜀 +1

2*𝜎𝜀 + 𝐶𝑜𝑛𝑠𝑡𝑎𝑛𝑡. * (3.8)

2
*3.1.2.2 Computational Theory *

In linear elastic problems, 𝜎𝑖𝑗 = 𝐶𝑖𝑗𝑘𝑙𝜀𝑘𝑙*, where the elastic moduli tensor 𝐶*𝑖𝑗𝑘𝑙* is *
constant, and stress and strain are linearly related.

However, in linear viscoelastic problems,

𝜎𝑖𝑗 𝑡 = 𝜀𝑘𝑙_{0}𝑡 𝑡 − 𝑠 𝐶 𝑖𝑗𝑘𝑙 𝑠 𝑑𝑠= 𝐶𝑖𝑗𝑘𝑙_{0}𝑡 𝑡 − 𝑠 𝜀 𝑘𝑙 𝑠 𝑑𝑠*, * (3.10)
where 𝐶_{𝑖𝑗𝑘𝑙}* 𝑡 is moduli tensor at time t and i, j, k, l = 1, 2, or 3. It can be seen that the *
relation between stress and strain is history dependent. Thus to solve viscoelastic
problems, the energy expression becomes complicated and time steps are used. Using
the concept of time steps, the continuous eq. (3.10) can be rewritten as

𝜎_{𝑖𝑗} 𝑡_{𝑛} = 𝜀_{𝑘𝑙} 𝑡_{𝑛} 𝐶_{𝑖𝑗𝑘𝑙} 𝑡_{0}
+ 𝜀_{𝑘𝑙} 𝑡𝑘 [𝐶𝑖𝑗𝑘𝑙 𝑡𝑛 − 𝑡𝑘 −
𝑘=𝑛−1
𝑘=0
𝐶_{𝑖𝑗𝑘𝑙} 𝑡𝑛 − 𝑡𝑘+1 ],
(3.11)

where 𝑡0 is the initial time when load is applied and 𝑡𝑖* is the time at ith time step . *
Since in this program, time steps are set to be equal to each other, eq. (3.11) can
be simplified as
𝜎_{𝑖𝑗} 𝑡𝑛 = 𝜀𝑘𝑙 𝑡𝑛 𝐶𝑖𝑗𝑘𝑙 𝑡0
+ 𝜀𝑘𝑙 𝑡𝑘 [𝐶𝑖𝑗𝑘𝑙 𝑡𝑛−k −
𝑘=𝑛−1
𝑘=0
𝐶𝑖𝑗𝑘𝑙 𝑡𝑛−𝑘−1 ].
(3.12)

From eq. (3.12), it can be seen that to calculate the stress for each time step, the material properties and the displacements history should all be stored in the program for calculation, which is a computationally demanding task.

After modifying the equation for calculating stress, the expression for calculating the energy gradient, 𝑔𝑏, becomes

𝑔𝑏 = 𝑢 𝑡_{𝑛} 𝐴 𝑡_{0} + 𝑘=𝑛−1𝑢 𝑡_{𝑘} [𝐴 𝑡_{𝑛−𝑘} −

𝑘=0 𝐴 𝑡𝑛−𝑘−1* ] + b(𝑡*𝑛*)， * (3.13)
*where b(𝑡*_{𝑛}*) is obtained from the boundary conditions depending on the stiffness *

properties of the materials at time 𝑡𝑛.

*In eq. (3.13), since displacements from previous time steps are fixed, gb becomes *
a linear equation with respect to 𝑢 𝑡_{𝑛} , and the equation can be solved in the same way
as in elastic case. Eq. (3.13) can be rewritten as

𝑔𝑏 = 𝑢 𝑡_{𝑛} 𝐴 𝑡1 + 𝑏(𝑡𝑛), (3.14)

where 𝑏 𝑡𝑛 contains all the fixed components in eq. (3.13) at time equals 𝑡𝑛. After modifying the ELAS3D program by incorporating time steps and

modifying the equations of energy, boundary conditions, energy gradient and stress, the program can be used to solve viscoelastic problems.

**3.2.2 Flow Chart **

The procedural flow chart for the linear viscoelastic program is shown in Figure 10.

*Figure 10 Flow Chart for linear viscoelastic model. *

**YES **

**NO **
**Set time step t=1 **

**Input basic information of the **
**material and calculate all necessary **
**matrixes at t [A(t**n**), b(t**n**), C(t**n**)] **

**Calculate energy using **
**all u(t**n**) **

**Set initial displacement for **
**each node at t u(t**n**) **

**Is energy at t**n

**minimized? **

**Store the displacement u( t**n **), **

**calculate and output modulus E(t**n**) **

**Change the values of **
**displacements u(t**n**) **

**END **
**Have all time steps **
**been calculated? **

**Increase time step by **
**1 **

**NO **

**3.3 Dissolution and Formation **

**3.3.1 Theory **

Both hydration and viscoelastic behavior are history dependent behavior, thus time steps should also be used to numerically account for history effects of dissolution and formation processes.

The process of dissolution and formation can be divided into several steps illustrated conceptually in Figure 11:

*Figure 11 Conceptual diagram of computational model simulating apparent viscoelastic *
*behavior of hydrating cement paste where 𝜎 is a constant applied external macroscale *
*stress and t is time elapsed. *

In Figure 11, the steps are:

(a) Before load is applied and there are a certain amount of load-bearing unhydrated materials phases;

(b) Load is applied and inherent components deforms under stresses;

(c) After some time, some unhydrated material dissolves, increasing the stress in surrounding phases. Inherent stress and strain redistribute to maintain the

boundary condition and the overall deformation of the composite microstructure changes.

(d) New components form in the deformed configuration with free strain and no stresses;

The main challenge in dealing with dissolution-formation problem is that after formation occurs, no historical behavior before formation should be considered and free strain is produced inside microstructure. That is, newly formed phases form in stress-free state that conforms to the preexisting deformed geometry. Thus to correctly predict the behavior of such materials, information regarding free strain and the time at which aging occurs should all be stored in the program.

The energy gradient can still be written as a linear equation

𝑔𝑏 = 𝑢 𝑡_{𝑛} 𝐴 𝑡_{0} − 𝑢_{𝑓}𝐴 𝑡_{0} + 𝑏 𝑡_{𝑛} , (3.15)
where 𝑏 𝑡𝑛 contains the values calculated from periodic boundary conditions, values
calculated from viscoelastic histories, and 𝑢_{𝑓} is the free strain.

𝑔𝑏 = 𝑢 𝑡𝑛 𝐴 𝑡0 + 𝑏 𝑡𝑛 , (3.16) where 𝑏 𝑡𝑛 contains all the fixed variables at time equals 𝑡𝑛, including the values calculated from periodic boundary conditions, values calculated from viscoelastic histories, and values calculated from free strains.

Some modifications should also be made to the energy equation and to the constitutive equation. The overall process is similar with the process of linear viscoelastic problems.

**3.3.2 Flow Chart **

The procedural flow chart for the dissolution-formation viscoelastic program is shown in Figure 12.

*Figure 12 Flow Chart for dissolution-formation viscoelastic model. *

**YES **

**YES **

**NO **
**Set time step t=1 **

**Calculate ** **and ** **modify ** **stiffness **
**matrixes [A(𝐭)] for all time steps, and **
**calculate b(𝐭**_{𝐧}**), C(𝐭**_{𝐧}**)] **

**Calculate energy using **
**modified strain. **

**Set initial displacement for **
**each node at t u(𝐭**𝐧**) **

**Is energy at 𝐭**𝐧
**minimized? **

**Change the values of **
**displacements u(𝐭**𝐧**) **

**Increase time step by 1 **
**Store the displacement u(t**n**), calculate **

**and output modulus E(𝐭**𝐧**) **

**END **
**Have all time steps **
**been calculated? **

**Input basic information of the material and **
**compare the phase of each voxel **

**Does the phase change? ** **Modify the modulus E **
**for all time steps **

**Record the strain in **
**each ** **pixel ** **before **
**formation in matrix U0. **

**YES **

**NO **

**NO **
**vo **

CHAPTER IV

RESULTS AND DISCUSSION

In this chapter, the results from the dissolution-formation viscoelastic program are shown in graphs, and discussion about these results will be presented. First, the validation of the program is checked, and then detailed analysis and comparisons of the results are presented to gain a deeper understanding towards the mechanisms of the viscoelastic behavior of cement paste. Equation Chapter (Next) Section 1

**4.1 Validation of Model **

**4.1.1 Elastic **

Elastic cases were tested for the dissolution-formation viscoelastic program at the first step, and the results from the program were compared with the results from the ELAS3D model and Abaqus.

First, since the dissolution-formation viscoelastic program in this thesis was a modification based on the NISTIR ELAS3D program, which was developed by

Garboczi et al. [1], results from the dissolution-formation viscoelastic program were first compared with the results from the NISTIR ELAS3D program for elastic cases. The purpose of this procedure was to make sure that the translation from FORTRAN to C++ was correct, and there were no errors in the elastic part of the program.

Next, the results from the dissolution-formation viscoelastic program were compared with the results from the program Abaqus. Abaqus is a well-known

behavior of materials. By checking the results from the program with the results from Abaqus, the accuracy of the program can be further ensured.

Figure 13 shows the comparison results from the three programs: NISTIR ELAS3D, Abaqus and the dissolution-formation viscoelastic program developed in this thesis.

*Figure 13 Comparison of elastic results from the dissolution-formation viscoelastic *
*program, the NISTIR ELAS3D program and the Abaqus program for cement paste with *
*w/c of 0.40 and 0.45 at different loading ages. *

14 16 18 20 22 24 0 1 2 3 4 5 6 7 8

The Aging viscoelastic program

NISTIR ELAS3D ABAQUS You ng' s M o dul us(GPa) Time(Days)

It can be seen from Figure 13 that the results from the three programs match with each other, and the accuracy of elastic part of the dissolution-formation viscoelastic program can be guaranteed.

**4.1.2 Viscoelastic **

For the viscoelastic part of the dissolution-formation viscoelastic program, first the results from the program for some special cases were checked. Second, the results from the program were compared with the results from Abaqus on non-aging linear viscoelastic composite materials.

Since the model is a composite materials model, for some simple cases, the results from the program can be compared with analytical results. For example, if all components of the composite carry the same material phases, the final modulus of the whole microstructure should be the same as the modulus of this material. The

dissolution-formation viscoelastic program showed satisfying results for these special cases.

Second, the viscoelastic results from this program were also compared with the results from Abaqus for simple random non-aging composites. A random three

dimensional non-aging composite matrix with the dimension 20 by 20 by 20 was

*generated in a Mathematica program, and then this composite matrix was analyzed with *
assigned component properties in Abaqus. The same matrix and component properties
were used in the dissolution-formation viscoelastic program and the results from these
two programs were compared. Figure 14 shows the comparison results, and there are
consistencies between these two programs for the simple non-aging matrix.

*Figure 14 Comparison of viscoelastic results from the dissolution-formation viscoelastic *
*program and the Abaqus program, where phases are either elastic or linear viscoelastic *
*and microstructure is unchanging. *

**4.1.3 Dissolution-Formation **

Currently, there are no valid ways of checking the accuracy of the dissolution-formation part of this viscoelastic model. However, to confirm the accuracy of the dissolution-formation part of the program, some simple special cases were tested.

The main difficulty for predicting the dissolution-formation process is the stress redistribution after the dissolution of existing load bearing phases and the formation of stress-free solidified phases. To prove this dissolution-formation viscoelastic program can give realistic simulation at this part, a simple virtual test was carried out.

41 42 43 44 45 46 47 48 0 2 4 6 8 10 12

The Dissolution-Formation Viscoelastic program Abaqus

Viscoel

astic Young's Modul

us E(t

) (GPa)

Consider an example where there is one cement composite matrix, and the C-S-H
phase inside it is assigned a viscoelastic Young‟s modulus of 11.2 + 11.2𝑒−0.2𝑡_{ , where }
*t is in days, and a constant Poisson‟s ratio of 0.25, while all other components of the *
composite material are assumed to carry the same elastic properties as shown in Table 1.
Then a virtual strain history shown in Figure 15 is applied on this composite. During the
first 13 days, a constant bulk strain of 0.1 is applied on the composite material, and at the
13th day, there is a sudden removal of the strain and the material is forced to return back
to its original dimension of zero bulk strain.

*Figure 15 Virtual applied strain history. *

-0.02 0 0.02 0.04 0.06 0.08 0.1 0.12 0 5 10 15 20 25 30 Applied Strain Appli ed Strain Time (Days)

bulk stress predicted by the dissolution-formation viscoelastic model is shown in Figure 16, where bulk stress is defined as

𝐴𝑝𝑝𝑎𝑟𝑒𝑛𝑡 𝑉𝑖𝑠𝑐𝑜𝑒𝑙𝑎𝑠𝑡𝑖𝑐 𝐵𝑢𝑙𝑘 𝑆𝑡𝑟𝑒𝑠𝑠 =𝜎11+ 𝜎22 + 𝜎33

3 . (4.1)

*Figure 16 Response of aging viscoelastic composite material when a strain history *
*shown in Figure 15 is applied. *

It can be seen from Figure 16 that during the first 13 days, the composite showed relaxation under the constant controlled strain. At the 13th day, the strain was suddenly forced back to zero and this induced a sudden change in the response of the material. The apparent bulk stress inside the composite dropped down significantly.

-1 0 1 2 3 4 5 6 0 5 10 15 20 25 30

Permenant Stress at Zero Strain Apparent Stress

Appare

nt

Vi

scoelastic Bulk Stress (GPa)

One interesting thing is that, after the strain went back to zero, the stress in the material did not go back to zero but turned into an opposite value. That is if the

composite was under compression during the first 13 days, it would suffer tension after the total stain was forced back to zero. Similarly, if the material suffered tension during the first 13 days, it would experience compression after the 13th day. For materials that have new solids forming as time evolves, this makes sense because of the existence of free strain that arises out of the need for new phases to form in a stress-free state.

When a controlled strain was applied, the inherent components carried stresses and deformed. During the hydration process, some components inside the composite material dissolved and formed new components. These new components formed in the deformed configuration without carrying any stresses and this unstressed deformation was strain free. Thus, when the bulk strain of the microstructure was forced back to zero, there were opposite stresses from these components. After the sudden change of strain, the responses of the material went back to relaxation again and resulted in a permanent stress, as shown in Figure 16.

**4.2 Viscoelasticity of C-S-H and Hydration **

As discussed in Chapter 2, both viscoelasticity of C-S-H and the hydration

process may play an important role in determining cement paste‟s viscoelastic properties. The dissolution-formation viscoelastic program makes the comparison of these two aspects possible and the comparison results are shown in detail in this section. Through

viscoelastic properties of cementitious materials.

All the following results in this chapter are obtained through running the dissolution-formation viscoelastic program on the microstructures generated by

THAMES on cement pastes of CCRL Proficiency Sample 168. The pastes are modeled
as hydrated at 25℃ (298K) under sealed moisture conditions with different w/c ratios
[27]. The sizes of these microstructures are 100 voxels by 100 voxels by 100 voxels,
with each voxel 1 𝜇𝑚3_{. }

By applying controlled pure volumetric stress and pure shear stress on theses 100 voxels by 100 voxels by 100 voxels microstructures, apparent viscoelastic Bulk modulus and apparent vicoelastic Shear modulus can be obtained. With known apparent

viscoelastic Bulk modulus and apparent vicoelastic Shear modulus, using Laplace Transform, apparent viscoelastic Young‟s modulus and apparent Poisson‟s ratio can be calculated.

Laplace Transform transforms expressions of apparent viscoelastic moduli from time-domain to frequency-domain. Meanwhile, Laplace transformation of the

constitutive equation for linear isotropic viscoelasticity has the same form as that for
*linear elasticity when multiplying each parameter by s, where s is the changing variable *
in frequency-domain. Thus the relation between the four viscoelastic moduli in

frequency-domain becomes:

𝑠𝐸 = 9𝑠𝐾 𝑠𝐺

3𝑠𝐾 + 𝑠𝐺 𝑠𝜈 =

3𝑠𝐾 − 2𝑠𝐺

where 𝐸 , 𝐾 , 𝐺 , 𝜈 are the Laplace transformation of apparent viscoelastic Young‟s modulus, apparent viscoelastic Bulk modulus, apparent viscoelastic Shear modulus and apparent viscoelastic Poisson‟s ratio. After obtaining the expressions for apparent viscoelastic Young‟s modulus and apparent viscoelastic Poisson‟s ratio in frequency-domain, they can be transferred back to time-domain for plotting.

Another way of calculating apparent viscoelastic Young‟s modulus and apparent viscoelastic Poisson‟s ratio with known apparent viscoelastic Bulk modulus and

apparent viscoelastic Shear modulus is by using time steps. The continuous time in constitutive equation for linear viscoelasticity can be separated into discrete time steps and apparent viscoelastic Young‟s modulus and apparent viscoelastic Poisson‟s ratio at each time step can be calculated with known apparent viscoelastic Bulk modulus and apparent viscoelastic Shear modulus from all previous time steps.

These two different calculation methods give the same results.

**4.2.1 Viscoelasticity of C-S-H **

In this section, the viscoelastic Young‟s modulus for 1 day old cement paste and 28 day old cement paste were compared. The 1 day old viscoelastic Young‟s modulus was generated by utilizing the 1 day old microstructure and the 28 day old viscoelastic Young‟s modulus was generated by utilizing the 28 day old microstructure. In this way, only the viscoelastic properties of C-S-H dominated the viscoelastic Young‟s modulus results, and there was no microstructure change of the composite inside the

for modeling creep or relaxation of the C-S-H phase over several days, for example as
the experiments shown in Figure 8, which last only 30s. Therefore, for simulation
purposes, the viscoelastic Young‟s modulus of C-S-H was assumed to be 11.2 +
11.2𝑒−0.2𝑡* _{, where t is in days and the Poisson‟s ratio of C-S-H was set to be a constant }*
value of 0.2. The elastic properties of all other phases were taken from Table 1.

The responses of the cement paste are shown in Figure 17.

*Figure 17 Viscoelastic Young’s modulus for cement paste at different ages (1 day old *
*and 28 day old) when dissolution and formation effect is not considered for the total *
*viscoelastic behavior of cement paste. The viscoelastic Young’s modulus of C-S-H is *
*assumed to be 11.2 + 11.2𝑒*−0.2𝑡_{, where t is in days and the Poisson’s ratio of C-S-H is }*assumed to be a constant value of 0.2. The elastic properties of all other phases were *
*taken from Table 1. *

10 12 14 16 18 20 22 0 10 20 30 40 50 60 70 80 1 day old 28 days old Vis co ela sti c Yo ung 's M o dul us E(t) (GPa) Time(Days)

Figure 17 shows the viscoelastic response of cement paste due to the viscoelastic properties of C-S-H. According to the simulation results, a 28 day old cement paste would exhibit more relaxation than l day old cement paste. The reason behind the predicted higher relaxation for older materials is that as volume fraction of C-S-H increases with age, so do the magnitude of stresses transmitted by C-S-H. Therefore, if C-S-H is the only viscoelastic phase in cement paste, more C-S-H results in more relaxation or creep. However, these predictions are in contrast to experimental results, which shows that there is more relaxation in younger cement paste than in older materials[37, 38]. Thus, it appears that the inherent viscoelasticity of C-S-H cannot be the primary mechanism of cement paste viscoelasticity because its confliction with experimental evidence of reduction in viscoelastic relaxation with age. A further discussion of this issue will be shown in section 4.2.3.

The solidification theory considers the forming of new phases but it does not include the dissolution of phases. The solidification theory implies that hydration products are non-aging viscoelastic materials and the amount of solidified products increases with time, as shown in Figure 4. The load bearing materials increase with time as a result of solidification and deposition of hydration products. However, in reality, formation of new load bearing phases requires dissolution of existent loading bearing phases, which is not included in the solidification theory. As a result of increasing amount of load bearing phases in the solidification theory, the stress carried by new loading bearing phases is gradually decreasing, and cement paste at later age will show less relaxation because of the decreasing inherent averaged stress, which is different

theory and the dissolution-formation viscoelastic program will be shown in later sections.

**4.2.2 Viscoelasticity of C-S-H and Dissolution **

When examining both effect of dissolution of load bearing phases and C-S-H
*viscoelasticity, different results were shown from Figure 17. *

As mentioned in chapter 3, discrete time steps were used in the dissolution-formation viscoelastic program, time steps representing different ages of the whole composite material. When time equals 1 day in the program, microstructure at 1 day old was input into the program. As program runs, time steps increases. When time increases to 1.5 day, the 1.5 day old microstructure was input into the program for analysis instead of the 1 day old microstructure. In the end, all microstructures would be analyzed and the progress of dissolution of unhydrated phases can be accounted for by applying these different microstructures. 0.4 w/c microstructures from 1 day to 4.5 days were used to generate Figure 18, which shows the predicted results when examining both effect of dissolution of load bearing phases and inherent C-S-H viscoelasticity.

*Figure 18 Response of cement paste with an assumed viscoelastic Young’s modulus of *
*C-S-H comparing to the response of cement paste when C-S-H is considered elastic. The *
*viscoelastic Young’s modulus of C-S-H is assumed to be 11.2 + 11.2𝑒*−0.2𝑡_{, where t is in }*days and the Poisson’s ratio of C-S-H is assumed to be a constant value 0.25. The *
*elastic properties of all other phases were taken from Table 1. *

In Figure 18, the solid line shows the response when C-S-H is considered to be
an elastic material, and the dashed line shows the response when C-S-H is treated as
viscoelastic. The C-S-H phases were assumed to be the only viscoelastic phase in
cement paste with the assumed viscoelastic Young‟s modulus 11.2 + 11.2𝑒−0.2𝑡_{, where }
*t is in days, and the Poisson‟s ratio was set to be a constant 0.25. *

From Figure 18, it can be seen that, the main trend of the viscoelasticity of cement paste is partially determined by the dissolution effect as well as the

12 13 14 15 16 17 18 0.5 1 1.5 2 2.5 3 3.5 4 4.5 Elastic Viscoelastic Appare nt Vi scoelastic Young 's Mo dulus E(t) (G Pa ) Time (Days)

with time.

**4.2.3 Mechanisms of Viscoelasticity of Cement Paste **

As mentioned, if the C-S-H phase shows a significant amount of relaxation, viscoelasticity of C-S-H contributes to the viscoelasticity of the whole microstructure. However, from the simulation results of the dissolution-formation viscoelastic program, another main reason leading to the viscoelastic property of cement paste is the

dissolution of load bearing phases.

Another finding by the dissolution-formation viscoelastic program is that even if viscoelasticity of C-S-H can contribute to the viscoelasticity of the whole microstructure, it cannot be the main mechanism leading to the viscoelastic behavior of cement paste. The only way that C-S-H viscoelastic deformation could be the dominant mechanism would be that if the dominant aging mechanism were inherent aging of C-S-H rather than the hydration process. That is, the viscoelastic properties of C-S-H would need to be dramatically evolved with the age of C-S-H particles.

Further experiments are needed to clearly determine the properties of C-S-H over a broader time scale.

**4.3 Predicted Effect of Different Loading Ages **

**4.3.1 Apparent Viscoelastic Young’s Modulus **

It is known that the responses of aging viscoelastic materials depend significantly on loading histories. If loads are applied at different ages, the responses would be

different. This section shows the predicted responses of cement paste at different loading ages (1 day and 7 days) by the dissolution-formation viscoelastic program.

Figure 19 shows the predicted apparent viscoelastic Young‟s modulus of 0.40 w/c paste with different loading ages of 1 day and 7 days. All phases in the composite were assumed to be elastic and the results were generated using the microstructures from 1 day to 56 days. For loading age of 1 day, microstructures from 1 day to 56 days were used and boundary conditions were applied starting from the 1st day microstructure. For loading age of 7 days, microstructures from 7 days to 56 days were used and boundary conditions were applied starting from the 7th day microstructure. The elastic properties of the components inside the composite material were taken from Table 1, including C-S-H. In this way, only the effect of dissolution was considered, and the relaxation was due entirely to dissolution effects.

*Figure 19 Apparent viscoelastic Young’s modulus of 0.40 w/c paste when loaded at *
*different ages. In this graph, apparent viscoelasticity is considered to occur strictly due *
*to dissolution of load bearing phases *

Cement paste will generate a higher elastic Young‟s modulus when loaded at a later age. This is because, when loaded at a later age, as hydration process goes on, more and more water and cement react into C-S-H and CH, which is also called the process of solidification. During this process, the cement paste becomes stiffer and stiffer because of increasing interparticle connections and reduced porosity.

To examine the effect of loading ages on rate of relaxation, data from Figure 19 were normalized by instantaneous apparent viscoelastic Young‟s modulus to get Figure 20. 12 14 16 18 20 22 24 0 10 20 30 40 50 60

Load is applied at 1st day

Load is applied at 7th day

App aren t Vis co ela sti c Yo ung 's M o dul us (G Pa ) Time(Days)